ViaFix

Instructions
Gebrauchsanweisung
Mode d’emploi

#50300110
2016.11.01

English
Description

ViaFix is a two component acrylic mounting system, consistingof one powder and one liquid. ViaFix is ideal for filling vias andmicroscopic voids, i.e. blind vias and microvias.
The system cures at room temperature. To obtain the clearest
mount the use of a pressure chamber is recommended.
ViaFix is affected by alcohol. We recommend using DiaPro forpreparation. The use of diamond products or lubricants
containing alcohols will affect the surface and the polymer willappear darker. We also recommend cleaning the specimen withwater and soap. When using cotton wool with alcohol forcleaning, there will be a risk of smearing the resin over thespecimen.

Safety Data Sheet

Please download a copy of the Safety Data Sheet from theLibrary section on www.Struers.com and read carefully beforeuse.
Access the Struers Library from the top menu on the website.

Please check the Library periodically for updates to the Safety
Data information.

StorageAcrylic powders absorb moisture. For maximum shelf life, store
ViaFix Powder under dry and cool conditions less then 20°C /68°F.
Acrylic liquids are sensitive to temperature. For maximum shelflife, store ViaFix Liquid under dry and cool conditions between
0°C / 32°F and 20°C / 68°F.

Mounting ofSpecimens
Measuring ofComponents

The ratio for ViaFix Powder:ViaFix Liquid is 11:9 by weight and2:1 by volume. Weighing is recommended to obtain the best
mounts and for reproducibility.
Important!
Do NOT pour excess liquid back into the bottle as this will
significantly reduce the shelf-life.

Mixing ofComponents Measure out the amount of ViaFix Powder into a mixing cup(max. 55 g / 5 x 20 ml).
 Measure out the amount of ViaFix Liquid into a mixing cup(max. 45 g / 5 x 10 ml).
 Sprinkle the powder into the liquid while stirring.
 Stir thoroughly until the mixture is homogeneous, without

introducing air bubbles into the mixture.
Immediately after the components are mixed polymerisationof the resin starts and the viscosity will increase. To get thebest filling use the resin as soon as possible after mixing.

Selecting theMounting Cup

All Struers mounting cups can be used.

Pre-treatment ofspecimens

Ensure that the specimens are thoroughly cleaned and dry prior
to mounting. Each surface must be free from grease, moistureand other contaminants to promote the best possible adhesionof ViaFix to the specimen.

Mounting

 Place the cleaned specimen in the centre of the mounting

cup, mix the necessary amount of resin and carefully pourover the specimen.
 Ensure that no air remains trapped within cracks or cavities inthe specimen by moving the specimen or by tapping themounting cup on the table.

CuringViaFix is a room temperature curing system. For a 30 mm dia.
mount, the curing time is about 20 minutes. It is recommended
to always use a pressure chamber in order to obtain a clear
mount with no air trapped within the resin. When using apressure chamber the temperature in the chamber will normallyrise during curing, especially if many mounts are cured at thesame time. We recommend keeping the mount in the mounting
cup until the temperature is below 30°C/86°F. Above thistemperature the mount is soft, the surface sticky and is difficult
to take out of the cup.
When specimens with thin layers (d 2 mm) are mounted withViaFix, the mount must be cured at 40°C/104°F.

After Curing

After removal from the mounting cups, the mounts are
immediately ready for preparation. The top surface of the mountwill be rubbery for approx. 24 hours. If the mounts are preparedas single specimens the top surface must either be ground forapprox. 10 s on #220 SiC-paper or covered by a plastic Dymo®
or the like to prevent the pressure feet from sticking to themounts.
NB! Remember that ViaFix is affected by alcohol.

Technical Data
Components
ViaFixRatio
by weight

Ratio
by volume

ViaFix Powder

112

ViaFix Liquid91

NB For the best mount use weighing method.

Density

ViaFix Powder:
ViaFix Liquid:

0.71 g/ml
0.89 g/ml

CuringCan be prepared(ground and polished) after:

20 min.

Peak temperature:

115°C / 240°F

Pot life:

2 min.

30 mm dia. mounting cup without specimen at 21°C / 70°F.

Properties afterCuringHardness:
Density:

83 Shore D
1.1 g/ml

Colouring

ViaFix can be coloured with EpoDye (fluorescent dye) andAcryDye.

Tips− Some materials have very poor adhesion to acrylics which

can result in a gap between the specimen and resin. To
minimise this gap the mount can be refilled with ViaFix after
the first preparation cured in pressure chamber and preparedagain.

DeutschBeschreibung

ViaFix ist ein Zwei-Komponenten-Acrylharz Einbettmittel mit
niedriger Viskosität. Es besteht aus einem Pulver und einer
Flüssigkeit. ViaFix ist ideal zum Füllen von Vias undmikroskopisch kleinen Hohlräume, wie z.B. Blindvias undMikrovias.
Das System härtet bei Raumtemperatur aus. Um klare,
durchsichtige Einbettungen zu erzielen wird die Verwendungeines Drucktopfes empfohlen.
ViaFix wird von Alkohol angegriffen, deshalb empfehlen wir
DiaPro für die Präparation. Werden Diamantsuspensionen undSchmiermittel mit Alkohol verwendet wird die Oberfläche
angegriffen und der Kunststoff wird dunkel. Wir empfehlen auchdie Probe mit Wasser und Seife zu reinigen, da beim Reinigen
mit Alkohol und Watte die Gefahr besteht, dass das Einbettharzüber die Probenoberfläche geschmiert wird.

Sicherheitsdatenblätt

Bitte laden Sie eine Kopie des Sicherheitsdatenblattes vonder Struers Webseite www.Struers.com unter „Bibliothek“
herunter und lesen es vor Gebrauch sorgfältig durch.
Bibliothek finden Sie oben rechts auf der Webseite.

Bitte überprüfen Sie die Bibliothek regelmäßig auf Updates fürdie Sicherheitsdatenblätter.

Aufbewahrung

Acrylpulver nehmen Feuchtigkeit auf. Aus diesem Grunde
empfehlen wir, das Pulver kühl und trocken zu lagern (unter20°C); dadurch wird die maximale Verwendungsfähigkeit
erzielt.
Acrylflüssigkeiten sind temperaturempfindlich. Aus diesem
Grunde empfehlen wir, die Flüssigkeit kühl und trocken zulagern (zwischen 0 °C und 20 °C); dadurch wird die maximale
Verwendungsfähigkeit erzielt.

Einbetten derProben
Komponenten
abmessen

Nach Gewicht ist das Verhältnis 11:9 von ViaFix Pulver: ViaFix
Flüssigkeit und 2:1 nach Volumen. Es wird empfohlen dieMengen abzuwiegen, das ergibt die besten Einbettungen undgute Reproduzierbarkeit.
Wichtig!
Gießen Sie überschüssige Flüssigkeit NICHT in die Flaschezurück. Die Haltbarkeitsdauer wird dadurch wesentlichverringert.

Komponentenmischen

 Die ViaFix Pulvermenge abmessen (max. 55 g / 5 x 20 ml)

und in einen Mischbecher geben.
 Die ViaFix Flüssigkeitsmenge abmessen (max. 45 g /5 x 10 ml) und ebenfalls in den Mischbecher geben.
 Hinweis: Das Pulver nicht auf einmal in die Flüssigkeit geben

sondern bei gleichzeitigem Rühren einstreuen.
 Gründlich rühren bis die Mischung homogen ist, aber ohne

gleichzeitig Blasen einzurühren.
Die Polymerisation des Einbettmittels beginnt sofort nachdem Mischen der Komponenten und die Viskosität erhöht
sich. Deshalb sollte man das Einbettmittel so schnell wie
möglich nach dem Mischen vergießen.
Einbettform
auswählen
Vorbehandlung derProben

Alle Struers Einbettformen können verwendet werden.
Sicherstellen, dass die Proben vor dem Einbetten gründlich
gereinigt und getrocknet werden. Die gesamte Oberfläche
muss frei von Fett, Feuchtigkeit und anderen Verunreinigungensein, um die best möglich Haftung von ViaFix an der Probe zuermöglichen.

Einbetten

 Die Probe in die Mitte der Einbettform legen, die notwendige

Menge von Einbettharz mischen und vorsichtig über dieProbe gießen.
 Indem man die Probe mit einer Pinzette etwas hin- undherbewegt, oder die Einbettform leicht auf die Tischplatte
klopft, stellt man sicher, dass keine Luftblasen in Rissen oder
Poren verbleiben.

Aushärtung

ViaFix härtet bei Raumtemperatur aus. Die Aushärtezeit füreine 30 mm Einbettform ist ungefähr 20 Minuten. Es wirdempfohlen immer einen Drucktopf zu verwenden damit dieEinbettung durchsichtig und ohne Luftblasen aushärtet. Bei derVerwendung eines Drucktopfes erhöht sich normalerweise
während der Aushärtezeit die Temperatur im Topf, besonders
wenn mehrer Proben gleichzeitig aushärten. Wir empfehlen dieEinbettungen in der Einbettform zu lassen bis die Temperatur
auf unter 30°C abgesunken ist. Oberhalb dieser Temperatur ist
die Einbettung weich und die Oberfläche noch klebrig und die
Einbettung lässt sich nur schwer aus der Form nehmen.
Beim Einbetten von Proben mit dünnen Schichten (< 2 mm),müssen die Einbettungen bei 40°C/104°F ausgehärtet werden.

Nach dem
Aushärten

Nach dem Herausnehmen aus der Einbettform können dieProben sofort präpariert werden. Die Oberfläche der Einbettung
ist für ca. 24 Stunden noch plastisch. Werden die Proben in
einem Halter für Einzelproben präpariert muss die Rückseite
entweder ca. 10 Sekunden mit SiC-Papier Körnung 220geschliffen werden, oder mit Dymo® Klebeband oderähnlichem abgedeckt werden, damit die Druckfüße desProbenbewegers nicht an der Einbettung hängen bleiben.
Hinweis! Bitte beachten Sie, dass ViaFix von Alkohol
angegriffen wird.

Technische Daten

ViaFix

Komponenten

Gewichtsverhältnis

Volumenverhältnis

ViaFix Pulver

112

ViaFixFlüssigkeit

91

NB Die besten Ergebnisse werden erzielt wenn die Mengen
abgewogen werden.

DichteViaFix Pulver:
ViaFix Flüssigkeit:

0.71 g/ml
0.89 g/ml

AushärtungKann präpariert werden (geschliffenund poliert) nach:

20 Min.

Spitzentemperatur:

115°C / 240°FTopfzeit

2 Min.

30 mm Durchm. Einbettform ohne Probe bei 21°C / 70°F

Eigenschaften
nach dem

Härte:
Dichte:83 Shore D
1.1 g/ml

FärbenViaFix kann mit EpoDye (fluoreszierender Farbstoff) oder
AcryDye gefärbt werden.

Tipps− Einige Werkstoffe haften sehr schlecht an Acrylharzen und es

kann sich ein Spalt zwischen Probe und Einbettmittel bilden.
Um diesen Spalt zu reduzieren kann man ihn nach der erstenPräparation mit ViaFix füllen, in einem Drucktopf aushärten
lassen, und danach die Probe noch einmal präparieren.

FrançaisDescription

ViaFix est un système d’enrobage acrylique à deuxcomposants, à faible viscosité, constitué d’une poudre et d’unliquide. ViaFix est idéale pour le remplissage des vias et desvides microscopiques, c’est à dire les vias masquées et lesmicrovias.
Ce système durcit à température ambiante. Pour obtenirl’enrobage le plus clair possible, l’utilisation d’une chambre depression est recommandée.
ViaFix est affectée par l’alcool. Nous recommandons l’utilisation
DiaPro pour la préparation. L’utilisation de produits diamantés
ou de lubrifiants contenant des alcools affecteront la surface etle polymère apparaîtra plus sombre. Nous recommandonségalement de nettoyer l’échantillon à l’eau et au savon. Lors del’utilisation d’ouate avec l’alcool pour le nettoyage, il peut yavoir un risque de beurrage de la résine sur l’échantillon.

Fiche de Sécurité

Télécharger une copie de la Fiche de Sécurité à partir de lasection Bibliothèque sur www.Struers.com et la lire avec
attention avant l’utilisation du produit.
L’accès à la Bibliothèque Struers se fait à partir du menu
supérieur sur notre site Web.

Vérifier la Bibliothèque à intervalles réguliers pour rester aucourant des mises à jour apportées aux Fiches de sécurité.

Conservation

Les poudres acryliques absorbent l’humidité. Pour une duréede vie en pot maximum, conserver la poudre ViaFix dans unendroit sec et frais (à moins de 20°C / 68°F).
Les liquides acryliques sont sensibles à la température. Pourune durée de vie en pot maximum, conserver le liquide ViaFix
dans un endroit sec et frais (entre 0°C / 32°F et 20°C / 68°F).

Enrobage deséchantillons
Mesure descomposantsLe taux est de 11:9 par poids de poudre ViaFix:Liquide ViaFix
et 2:1 par volume. La pesée est recommandée pour obtenir les
meilleurs enrobages et reproductibilité.
Important!
Ne PAS reverser l’excédent de liquide dans la bouteille, car celaréduira considérablement la durée de vie du produit.

Mélange descomposants

 Mesurer la quantité de poudre ViaFix dans un gobelet demélange (max. 55g / 5 x 20 ml).
 Mesurer la quantité de Liquide ViaFix dans un gobelet demélange (max. 45g / 5 x 10 ml).
 Saupoudrer la poudre dans le liquide tout en mélangeant.
 Mélanger soigneusement jusqu’à ce que le mélange soit

homogène, sans introduire de bulles d’air dans le mélange.
Immédiatement après le mélange des composants, lapolymérisation de la résine commence et la viscositéaugmente. Pour obtenir l’effet de remplissage le meilleur,utiliser la résine dès que possible après le mélange.
Choisir le mouled’enrobage

Tous les moules d’enrobage Struers peuvent être utilisés.

Pré-traitement deséchantillons

S’assurer que les échantillons soient soigneusement nettoyés
et secs avant l’enrobage. Chaque surface doit être exempte degraisse, humidité et autres substances contaminantes afind’assurer la meilleure adhésion possible de ViaFix àl’échantillon.

Enrobage Placer l’échantillon nettoyé au centre du moule d’enrobage,mélanger la quantité nécessaire de résine et verser avec
précaution sur l’échantillon.
 S’assurer qu’il ne reste pas d’air pris dans les fentes ou
cavités dans l’échantillon en déplaçant l’échantillon ou entapant le moule d’enrobage sur la table.

Durcissement

ViaFix est un système durcissant à température ambiante. Pourun moule de 30 mm de dia., le temps de durcissement est
d’environ 20 minutes. Il est recommandé de toujours utiliser
une chambre sous pression afin d’obtenir un enrobagetransparent sans aucun air pris dans la résine. Lors de l’emploi
d’une chambre sous pression, la température dans la chambre
augmentera normalement au cours du durcissement,particulièrement si de nombreux échantillons durcissent enmême temps. Nous recommandons le maintien de l’échantillon
dans le moule d’enrobage jusqu’à ce que la température soit
inférieure à 30°C/86°F. Au-dessus de cette température,l’enrobage est mou, la surface collante et l’enrobage est difficile
à retirer du moule.
Lorsque les échantillons à couches minces (d 2 mm) sontenrobés dans ViaFix, l’enrobage devra être durci à 40°C/104°F.

Après durcissement

Après leur retrait du moule d’enrobage, les échantillons sontimmédiatement prêts pour la préparation. La partie supérieurede la surface de l’enrobage sera caoutchouteuse pendantenviron 24 heures. Si les enrobages sont préparés commeéchantillons individuels, la partie supérieure de la surface devra
soit être prépolie pendant environ 10 s sur papier SiC de #220
soit ruban Dymo® ou similaire pour empêcher que le sabot depression d’adhére à l’enrobage.
NB! Se rappeler que ViaFix est affectée par l’alcool.

Données techniques
ComposantsViaFix

Tauxpar poids

Taux
par volume

ViaFix Poudre

112

ViaFix Liquide

91

NB Pour obtenir le meilleur enrobage, utiliser la technique de la pesée.

Densité

ViaFix Poudre:
ViaFix Liquide:

0,71 g/ml
0,89 g/ml

Durcissement
Peut être préparé
(prépoli et poli) après:

20 min.

Température de crête:115°C / 240°F

Durée de vie en pot:

2 min.

Moule d’enrobage de 30 mm de dia. sans échantillon à 21 °C / 70°F

Propriétés après
durcissement

Dureté:Densité:83 Shore D
1,1 g/ml

Coloration

ViaFix peut être colorée avec EpoDye (teinture fluorescente)et AcryDye.

Conseils− Certains matériaux montrent une très mauvaise adhésion auxacryliques ce qui peut résulter en une fente entre l’échantillon
et la résine. Pour minimiser cette fente, l’enrobage peut êtrede nouveau rempli avec ViaFix après que la première
préparation ait durcie dans la chambre de pression, puis êtrepréparé de nouveau.

Visit the Struers e-shop to see the latest additions to theStruers consumables range. www.e-shop.struers.com

Besuchen Sie den Struers e-Shop – hier finden Sie alleaktuellen Verbrauchsmaterialien und Informationen zu neuen
Produkten. www.e-shop.struers.com

Visitez notre boutique Struers e-shop pour vous tenir informédes dernières nouveautés Struers en matière deconsommables. www.e-shop.struers.com

Pederstrupvej 84, DK-2750 Ballerup